Synthesis and Growth Mechanism of Ni Nanotubes and Nanowires
© to the authors 2009
Received: 23 December 2008
Accepted: 14 May 2009
Published: 31 May 2009
Highly ordered Ni nanotube and nanowire arrays were fabricated via electrodeposition. The Ni microstructures and the process of the formation were investigated using conventional and high-resolution transmission electron microscope. Herein, we demonstrated the systematic fabrication of Ni nanotube and nanowire arrays and proposed an original growth mechanism. With the different deposition time, nanotubes or nanowires can be obtained. Tubular nanostructures can be obtained at short time, while nanowires take longer time to form. This formation mechanism is applicable to design and synthesize other metal nanostructures and even compound nanostuctures via template-based electrodeposition.
KeywordsNanotubes Nanowires Growth mechanism Electrodeposition
Nanostructures have received comprehensive attention owing to their novel optical, electrical, catalytic and magnetic properties and their potential applications in nanoscale electronic, sensing, mechanical and magnetic devices [1, 2], and information storage systems [3–6]. Among various synthetic processes, template synthesis has been proved to be a versatile and simple approach for the preparation of many nanostructures, such as conductive polymers, metals, semiconductors, carbon and other materials [7–10]. Among these materials, metal nanostructures have been the focus of extensive research activities due to their unusual properties . Many groups have focused on the magnetic properties of nickel (Ni) nanotubes and/or nanowires [12–15], because of their small magnetocrystalline anisotropy energy and potential application in devices. Some groups have studied the formation mechanism of the Ni nanostructures [16–21], but the growth mechanism is still unclear so far. Therefore, a complete understanding of the growth mechanism needs intense investigation. This has aroused our interest to explore the growth mechanism of Ni nanotubes and nanowires.
In our work, we not only report the successful fabrication of ordered Ni nanotube and nanowire arrays using anodic aluminum oxide (AAO) templates by changing electrodeposition conditions, but also propose a growth mechanism for Ni nanotubes and nanowires. The proposed growth mechanism for Ni nanotubes and nanowires in our work is different from others reported before and is easier for the readers to understand. The obtained Ni nanotubes are more likely to enable us to fix metals or semiconductors in order to achieve novel nanocomposites with unique physical properties, and the Ni nanowire arrays might have potential applications in the magnetic–electric devices.
Nanotubes and nanowires were synthesized using template-directed electrochemical deposition, an approach pioneered by Martin [7, 8]. In general, AAO films are formed by the electrochemical oxidation of aluminum. Depending on the type of anodization process and growth regime used, aluminum oxide membranes can be fabricated to contain nanopores with a wide range of diameters, lengths and interpore distances. To facilitate nanowire fabrication, commercially available aluminum oxide membranes, Whatman Anodisc 25, were used, with a nominal pore diameter ranging from 150 to 300 nm and depths ranging from 50 to 60 μm.
The side of the AAO membrane was sputtered with a layer of Au as a work electrode. In a tri-electrode electrochemical system, the Ni nanostructure arrays were produced in the template pores from a solution of 0.8 mol/L NiSO4·6H2O + 0.5 mol/L H3BO3 + 0.3 mol/L KCl by direct current electrodeposition. The electrodeposition was carried out using platinum as an anode and a calomel electrode as a reference electrode. Finally, the nanowire arrays were revealed by the removal of AAO in a 3 mol/L sodium hydroxide solution. Three samples were prepared under different electrodeposition conditions. They were labeled as sample 1 (applied voltage: −0.8 V, deposition time: 20 min, corresponding current: 0.03–0.11 mA), sample 2 (−0.8 V, 40 min, 0.03–0.19 mA) and sample 3 (−0.8 V, 60 min, 0.04–0.26 mA).
The morphology of the Ni nanostructure arrays was investigated using a JEOL JSM-6390LV SEM. The structure and microstructure of the Ni nanotubes and nanowires were investigated using a JEOL JEM-2000EX TEM. The specimen for TEM observation was prepared by evaporating a drop (5 μL) of the nanostructure dispersion onto a carbon-film-coated copper grid. The growth process of Ni nanotubes and nanowires was investigated using high-resolution transmission electron microscope (HRTEM).
Results and Discussion
It can be seen from Fig. 1 that there is a length distribution for the nanotubes and nanowires in each sample. This is due to the difference of barrier layer thickness at each pore and also due to the hydrogen evolution caused by water-splitting reaction . Ni2+ ions are reduced during the electrodeposition by the electrons tunneled through the barrier layer. However, the barrier layer at each pore could be branched differently during the thinning process of the barrier layer, resulting in different energy barriers for tunneling because of different barrier layer thickness . The number of tunneled electrons through an insulating layer decreases exponentially with the thickness of the insulating layer according to Bethe’s equation . Consequently, the rate of deposition becomes different at each pore.
From the TEM results, we conclude that the formation process of Ni nanowires begins with the formation of Ni nanotubes. Nanotubes were formed at first, and then Ni nanoparticles of the electrode stacked randomly in the tubes, until nanowires were formed. The formation process is revealed vividly in Fig. 2a. With the increase in deposition time, nanotubes disappear gradually, and the amount of nanowires increases further. However, nanotubes still exist despite of the increased deposition time, because Ni2+ions concentration in the margin region of the templates is low and can not be supplemented from the whole solution in time. So, Ni nanoparticles are not enough to fill the Ni nanotubes in time; therefore, Ni nanotubes still exist in the margin regions of the templates.
Figure 4b shows vividly the formation process of the nanowires. When Ni nanotubes are formed, the surface absorption energy of nanochannels decreases accordingly. When theE field is preferential, Ni nanoparticles begin to stack inside the tubes from the electrode surface until the nanotubes are completely filled, and nanowires are obtained.
In summary, nanoparticles stack inside the tubes to form nanowires when the E field reached a certain value. We have termed this growth mechanism brick-stacked wirelike growth (BSWG). Cao et al.  have proposed a current-directed tubular growth (CDTG) mechanism. They believed that metal nanotubes can be obtained at v∥ (growth rate parallel to current direction) » v⊥(growth rate perpendicular to current direction), while nanowires can be obtained at v∥ ≈ v⊥.. However, we think that it is difficult to define the competitive rates.
It is well known that Ni is a magnetic material with very small magnetocrystalline anisotropy energy . The crystallographic orientations of these nanoparticles are different, so the shape anisotropy of these nanoparticles is also different. The adjacent nanoparticles will repel each other, resulting in Ni nanoparticles being randomly arranged and the grains having different crystallographic orientations, as shown in Fig. 3c.
Our results fully demonstrate that magnetic materials can form nanotubes and nanowires under appropriate synthesis conditions. We believe that the BSWG mechanism can be applied to synthesize other magnetic metal nanostructures. Controlling the synthesis conditions, other metal nanostructures can be deposited in magnetic nanotubes to form novel nanocomposite materials.
In summary, highly ordered Ni nanotubes and nanowires have been fabricated by DC electrodeposition in the pores of AAO templates under the deposition voltage of −0.8 V. Ni nanotubes were obtained when the deposition time was less than 20 min, and the corresponding current was 0.03–0.11 mA, while Ni nanowire arrays were obtained when the deposition time was more than 40 min and when the current was more than 0.19 mA. Systematic HRTEM investigations demonstrate the formation process of Ni nanostructures, and the growth mechanism for Ni nanotubes and nanowires has also been explored. We believe that the BSWG mechanism can be applied for other magnetic nanostructures; especially, such metal nanotubes with open ends have a variety of promising applications, such as porous electrodes filled with ferromagnetic and nonmagnetic metals to fabricate magnetic multilayer nanostructure, or other materials to prepare novel nanocomposite materials with special magnetic, optical or electrical properties.
This work was financially supported by the National Natural Science Foundation of China (No. 50473012) and the Provincial Natural Science Foundation (No. Z2005F03).
- Kovtyukhova NI, Mallouk TE: Chem. Eur. J.. 2002, 8: 4354. C COI number [1:CAS:528:DC%2BD38XotVKhurk%3D] 10.1002/1521-3765(20021004)8:19<4354::AID-CHEM4354>3.0.CO;2-1View Article
- Patolsky F, Zheng G, Hayden O, Lakadamyali M, Zhuang X, Lieber CM: Proc. Natl. Acad. Sci. U.S.A.. 2004, 104: 14017. Bibcode number [2004PNAS..10114017P] Bibcode number [2004PNAS..10114017P] 10.1073/pnas.0406159101View Article
- Gudiksen MS, Lauhon LJ, Wang JF, Smith DC, Lieber CM: Nature. 2002, 415: 617. C; COI number [1:CAS:528:DC%2BD38XhsVCjsL4%3D]; Bibcode number [2002Natur.415..617G] 10.1038/415617aView Article
- Cui Y, Wei QQ, Park HK, Lieber CM: Science. 2001, 293: 1289. C; COI number [1:CAS:528:DC%2BD3MXmtFCrtrs%3D]; Bibcode number [2001Sci...293.1289C] 10.1126/science.1062711View Article
- Thurn-Albrecht T, Schotter J, Ka¨stle CA, Emley N, Shibauchi T, Krusin-Elbaum L, Guarini K, Black CT, Tuominen MT, Russell TP: Science. 2000, 290: 2126. C; COI number [1:CAS:528:DC%2BD3cXptVyis7k%3D]; Bibcode number [2000Sci...290.2126T] 10.1126/science.290.5499.2126View Article
- Liang HP, Guo YQ, Hu JS, Zhu CF, Wan LJ, Bai CL: Inorg. Chem.. 2005, 44: 3013. C COI number [1:CAS:528:DC%2BD2MXisFOnt7w%3D] 10.1021/ic0500917View Article
- Martin CR: Science. 1994, 266: 1961. C; COI number [1:CAS:528:DyaK2MXisl2lur0%3D]; Bibcode number [1994Sci...266.1961M] 10.1126/science.266.5193.1961View Article
- Martin CR: Chem. Mater.. 1996, 8: 1739. C COI number [1:CAS:528:DyaK28XkslKqu7c%3D] 10.1021/cm960166sView Article
- Huczko A: Appl. Phys. A. 2000, 70: 365. C; COI number [1:CAS:528:DC%2BD3cXisFyrur0%3D]; Bibcode number [2000ApPhA..70..365H] 10.1007/s003390051050View Article
- Peng K, Huang Z, Zhu J: Adv. Mater.. 2004, 16: 73. C COI number [1:CAS:528:DC%2BD2cXhtVaiuro%3D] 10.1002/adma.200306185View Article
- Pirota KR, Navas D, Hernandez-Velez M, Nielsch K, Vazquez M: J. Alloy Compd.. 2004, 369: 18. C COI number [1:CAS:528:DC%2BD2cXisl2lt7s%3D] 10.1016/j.jallcom.2003.09.040View Article
- Tian F, Zhu J, Wei D: J. Phys. Chem. C. 2007, 111: 12669. C COI number [1:CAS:528:DC%2BD2sXosVCrsbw%3D] 10.1021/jp0737294View Article
- Hangarter Carlos M, Myung Nosang V: Chem. Mater.. 2005, 17: 1320. 10.1021/cm047955rView Article
- Mousa MA, Imran J: Alloys Compd.. 2008, 455: 17. 10.1016/j.jallcom.2007.01.051View Article
- Shi JB, Chen YC, Lee CW, Lin YT, Wu C, Chen C: J. Mater. Lett.. 2008, 62: 15. C COI number [1:CAS:528:DC%2BD2sXhtlejsrzP] 10.1016/j.matlet.2007.04.060View Article
- Pan H, Liu BH, Yi JB, Poh C, Lim SH, Ding J, Feng YP, Huan CHA, Lin JY: J. Phys. Chem. B. 2005, 109: 3094. C COI number [1:CAS:528:DC%2BD2MXhtVKmsbk%3D] 10.1021/jp0451997View Article
- Jin CG, Liu WF, Jia C, Xiang XQ, Cai WL, Yao LZ, Li XG: J. Cryst. Growth. 2003, 258: 337. C; COI number [1:CAS:528:DC%2BD3sXns1Whtr8%3D]; Bibcode number [2003JCrGr.258..337J] 10.1016/S0022-0248(03)01542-2View Article
- Sellmyer DJ, Zheng M, Skomski R: J. Phys.: Condens. Matter. 2001, 13: R433. C; COI number [1:CAS:528:DC%2BD3MXlt1arsLo%3D]; Bibcode number [2001JPCM...13R.433S] 10.1088/0953-8984/13/25/201
- Tian F, Chen J, Zhu J, Apply J: Phys. 2008, 103: 013901.
- Cao HQ, Wang LD, Qiu Y, Wu QZ, Wang GZ, Zhang L, Liu XW: ChemPhysChem. 2006, 7: 1500. C COI number [1:CAS:528:DC%2BD28Xnt1Olu7s%3D] 10.1002/cphc.200500690View Article
- Wang QT, Wang GZ, Han XH, Wang XP, Hou JG: J. Phys. Chem. B. 2005, 109: 23326. C COI number [1:CAS:528:DC%2BD2MXht1Wmt7nK] 10.1021/jp0530202View Article
- Hwang SK, Jeong SH, Lee OJ, Lee KH: Microelectron. Eng.. 2005, 77: 2. C COI number [1:CAS:528:DC%2BD2cXhtVSiu73P] 10.1016/j.mee.2004.07.069View Article
- Sui YC, Cui BZ, Martı′nez L, Perez R, Sellmyer DJ: Thin Solid Films. 2002, 406: 64. C; COI number [1:CAS:528:DC%2BD38Xjt1Kju7o%3D]; Bibcode number [2002TSF...406...64S] 10.1016/S0040-6090(01)01769-2View Article
- Polymeropoulos EE: J. Appl. Phys.. 1977, 48: 2404. C; COI number [1:CAS:528:DyaE2sXksVOjsrY%3D]; Bibcode number [1977JAP....48.2404P] 10.1063/1.324002View Article
- Lahav M, Sehayek T, Vaskevich A, Rubinstein I: Angew. Chem.. 2003, 115: 5734. 10.1002/ange.200352216View Article
- Lahav M, Sehayek T, Vaskevich A, Rubinstein I: Angew. Chem. Int. Ed. Engl.. 2003, 42: 5576. C COI number [1:CAS:528:DC%2BD3sXpsl2ksrc%3D] 10.1002/anie.200352216View Article